Physica B 189 (1993) 225-234 North-Holland

*SDl 0921-4526(93)E0027-4*

**PHYSICA**

### Conductance and supercurrent discontinuities in atomic size

### point contacts

### CJ. Muller3, J.M. van Ruitenbeek3, C.W.J. Beenakkerb and R. de Bruyn Ouboter3

1*Kamerhngh Onnes Laboratory, bInstttuut-Lorentz, Umversity of Leiden, Leiden, The Netherlands*

A technique is descnbed, which uses the adjustable stress m a bendmg beam to control the constnction diameter
betwcen two electrodes The controllabihty of the constnction diameter is useful when a large ränge m the normal
resistance of different junctions is required for a systematic study In the high resistance point contact regirae quantum size
effects are studied m metallic and superconductmg constnctions When changmg the constnction diameter reproducible
*steps m the conductance of the order of 2e2Ih are observed For superconductmg point contacts concomitant jumps in the*
*supercurrent of order eAlh are seen For contacts adjusted at a step the conductance Switches m time between two values,*
which are interpreted äs "two level ffuctuations" m the site of a smgle atom m the constnction

**1. Introduction**

The conductance of a narrow contact under
the condition of ballistic motion of the electrons,
*changes by integer multiples of 2e2/h äs a *

func-tion of the width of the contact. This quantiza-tion of the conductance was discovered in point contacts of high mobility two-dimensional elec-tron gases in GaAs-AlGaAs heterostructures [1], having a large Fermi wavelength (AF — 400 Ä). Its explanation is based on the quantiza-tion of the transverse momentum of the elec-trons, which move through the contact. This principle is expected to apply to all wave phe-nomena. Indeed, also the transmission of light through a narrow aperture was subsequently discovered to be quantized [2]. Quantization of the conductance is now understood by means of the Landauer formalism [3]. The wave charactcr of the electrons, which manifests itself so strong-ly m the conductance of these mesoscopic struc-tures, should also show up in other transport properties. In particular, Beenakker and van Houten [4] predicted that the critical current of a

*Correspondence to· C l Muller, Kamerhngh Onnes *
Labora-tory, Umversity of Leiden, P O Box 9506, 2300 RA Leiden,
The Netherlands

short, impurity free superconductmg constriction
should increase stepwise äs a function of its
width. The step size was found to depend on the
superconducting energy gap,* Δ, äs eAlh.*

In principle, quantization of the conductance is also expected for point contacts of normal metals. This is more difficult to observe, how-ever, äs the Fermi wavelength in metals is of the order of the atomic diameter. To have constric-tion widths of the order of the Fermi wavelength implies that one should construct point contacts of atomic dimensions for which the diameter can be continuously adjusted. Variation of the con-striction diameter on such a fine scale will suffer from the limits set by the size of the atoms. Conduction quantization effects in metals will therefore be blurred by discrete atom-by-atom building up of the contact. Nevertheless, it is of considerable interest to study such small metallic point contacts. Some interesting questions to be investigated are: what is the number of quantum channels for conduction through one atom? How is this number related to the atomic shell struc-ture? Can we see the effects of conductance quantization? A metal point contact also offers the possibility to look for steps in the supercur-rent, a subject which is not yet accessible with semiconductor devices.

226 *C J Muller et al l Conductance and supercurrent discontmuttte^ m atomic size pomt contacts*

Here, an experimental method is described
which makes it possible to study atomic size
point contacts of any metal, and where the
contact size can be adjusted continuously. First
attempts at observing conductance quantization
in small normal metal and superconducting point
contacts are presented. When the point contact
constriction is increased the conductance is
ob-served to increase stepwise. The Steps are
inter-preted äs atom-by-atom increase of the contact
diameter. The step size for a platinum point
*contact is of order 2e2/h. In a niobium *

supercon-ducting point contact the steps in the normal state conductance are found to coincide with steps in the supercurrent, with a step size of the order of the predicted value [4].

In the next section the experimental tech-nique, which is used to obtain atomic size point contacts, is described in detail. Experiments on these contacts in the normal and the supercon-ducting state are presented in the last two sections. Parts of this paper have been published elsewhere [5,6].

**2. The experimental technique**

Here we describe an extension to Morelands
break junction technique [7], which is used to
obtain a clean and stable adjustable junction. A
crucial part in the setup is the sample mounting,
which is schematically drawn in fig. 1. A metal
filament of the material under investigation is
glued on a flexible glass bending beam, in such a
way that the central section remains unglued.
Prior to this procedure a notch is made in the
middle of the filament with a sharp scalpel. The
principle of Operation is to break the notched
part of the metal filament at liquid helium
temperatures, in vacuum, in order to obtain two
clean freshly broken electrodes. This is
estab-lished by bending the Substrate in a controllable
way, resulting in an elongation of the unglued
*section u. This elongation is concentrated on the*
weak notched part in the filament, and results in
the fracture, which is measured äs an abrupt
decrease of the conductivity to zero. After the
fracture of the electrodes the force, which acts

*PIEZO*

*EPOXY ADHESIVE*
*L- NOTCHED FILAMENT*

*•COUNTER SUPPORT*

*- BENDING BEAM*

Fig l A schematic drawmg of the sample mounting m a
three point bending configuration A force on the bending
beam, exerted via the piezo element, induces a small length
increase of the unglued section u to break the filament Once
this is estabhshed the force on the bending beam is used for
fine adjustment of a point contact or a tunnel junction The
*distance betwecn the counter Supports, l^, is approximately*
2cm

on the bending beam, is relaxed until the two electrode halves touch again. Once this is achieved the bending beam is still under a strain. By fine adjustment of the force acting on the bending beam, via a piezo element, it is possible to adjust atomic size point contacts or tunnel junctions with a subatomic vacuum distance äs the barrier.

*geome-C J Mulla et al l geome-Conduuance and <,upeiciiin'iit dnionliniutie'i in atomn \izc point* 227

**INHERENT STABLE DEVICES**

Fig 2 Two possible clectrode gcomctues The clccliodes are tightly conncctcd to thc bending bcam and foim an mheicntly stähle structuic In (a) Ihe two clcetiodes consti-lute a tunncl |unction, tunnelmg oecurnng somewheie be-twccn two ncaicst atoms on cithei side oi the clcan clcc-tiodcs In (b) Ihe two cleetrodes constitutc an atomic size point contact, wheic eleetion tiansport takes plaee via conduction.

try is the reason for the high stability of thc systcm and for the adjustability of the electrodcs over approximately 10~2 to IGT1 of an atomic

distance: a spccific length change of the piczo induccs an clectrode displacement, which is approximately a factor of thousand smaller. Due to thc breaking proccss of thc electrodc matcrial bcforc a junction can be established and becausc the junction resistancc is a controllable parame-tcr ovcr a large ränge, this dcvicc is callcd a mechanically controllable brcak (MCB) junc-tion.

Typical dimensions of the sample geomctry
*shown in fig. l arc: u — 0.1-0.3 mm and the*
distance betwccn the countersupports, /s — 2cm.

Fig. 3 shows a photograph of the ccntral section of thc sample mounting, aftcr it was used suc-cessfully in an experiment. The adjustment of the force on thc bending beam is performed by a coarse and a fine adjustment (see fig. 4). The

coarsc adjustment consists of spindle driven by an electromotor to move thc lever part towards the bending bcam. This adjustment is used to break the filament, and aftcr this to re-establish a contact by reversing the motor dircction. Once this is achieved a voltage on the piezo element is applied for fine adjustment of the constriction or the vacuum barrier between the electrodes. With this sctup two differcnt kinds of experiments are possible. In one kind of experiment the piezo voltage is kept constant, resulting in a junction with a specific rcsistance. In the other experi-ment the piezo voltage is continuously varied inducing a slowly varying resistance of the tion. This opcns the possibility to monitor junc-tion characteristics in a continuous mcasurement äs a function of the ]unction resistancc.

228 *C.J. Muller et al. l Conductance and supercurrent discontinuities in atomic size point contacts*

*W*

## v

J»\

### \

Fig. 3. An enlargcment of the central pari of the sample. The separated glue contacts arc clearly visiblc in the uppcr Icli photograph. An enlargcment of the notched part of the filament is shown in the other two photographs. The photos were taken aftcr successful Operation of the sample.

In the next section measurements are pre-sented in the contact regime, where the main attention is focussed on point contacts of atomic sizes. Unless stated otherwise the experiments have been performed in vacuum at 1.2 K.

**3. Point contacts of platinum**

As the measurements presented here are re-stricted to the contact regime, the maximum resistance, which can be obtained in this regime, is the resistance for a single atom contact. For a changing piezo voltage it is easy to deduce whether the junction is in the tunnel or contact regime, because the resistance changes smoothly in the tunnel regime, whereas in the contact regime Steps in the resistance occur äs a function

of piezo voltage. Experimentally we obtain a maximum resistance in the contact regime of about lükil.

The experiment with an increasing constriction
*diameter is shown in fig. 5, where two *
conduct-ance traces of the same platinum sample are
presented. Both traces show common features
although they do not reprouuce in detail, which
may be caused by somc piastic deformation in
the point contact region äs we scan the piezo
voltage, Vp. For a smaller ränge of Kp the fine

structure is reproducible äs will be shown below
for a niobium sample. Although we do not
observe conductance quantization, discontinuous
Steps in the conductance occur with a magnitude
*of the order of 2e2/h. When fixing the piezo*

*C.J. Muller et al. l Conductance and supercuirent discontmmlies m atomic size point contacfi* 229
*B C*

*J*

Fig 4. The mechanical adjustment pari in the vacuum chamber with; A: tubes for signal and piezo Icads containing copper powder filters, B: microwavc fccdthrough, C: spmdle, D: bcarings, E: fork-blade coupling, F· scrcw bolt, G: ball-keyholc coupling, H: lever, I: piezo element, J: sample mountmg, K: counter Supports, L: turning-point, M: copper rod.

Fig. 5. Two examples of traces of the conductance, G, äs a
function of decreasing piezo voltage, i.e., mcreasing
constric-tion diameter of a platinum sample. The füll scan was
recorded in about 20min. We estimate that 10V—1Ä.
*Conductance Steps are of the order of 2e2/h, but no *
quantiza-tion is observed. Curve a is offset in the horizontal direcquantiza-tion
with +10 V for clarity.

rcsistance states, where the switching frequency increascs with the bias. Fig. 6 shows this switch-ing effect between a 4.1 and 4.5 kfl state. An

*I-V characteristic of this switching contact, *

re-corded in O . l s , is shown in fig. 7. Similar switching behaviour between two levels, so-called two level fluctuations (TLFs), was ob-served by Ralls et al. [9] and Holweg et al. [10] in nano-constrictions with larger diameters com-pared to our atomic size point contacts.

From fig. 5 it is clear that the magnitude of the fluctuations can be äs large äs the conductance itself, moreover we are able to reproducibly create the TLFs and influence the duty cycle, i.e. the average time spent in one state divided by the total time. In the nano-structures of Ralls et al. and Hol weg et al. TLFs are believed to be

25 time(s) 50

*aHrt****·*
t

MtvV* VA kj

•Λ

1

Λλ

H*

*+ΛΙvor·*hH"|k
1 f

*r~J

0.5 time(s)

### VJ VJ

VJtime(ms) 10

time(ms) 10

Fig. 6. Time traces at different bias currents with the piezo
voltage tuned at a conductance Step, which Switches between
4.1 and 4.5 ΚΩ. The conductance change between upper and
lower level is the same in all panels, and is about 0.3* (2e2/h).*

230 *C / Muller et al l Conductance and supercurrent discontmuüies in atomic size pomt contacts*

0 _{V(mV)}_{ 50}
*Fig. 7 An l-V curve with the piezo voltage tuned at the*
same conductance step äs m fig 6 The total recordmg time
of this curve was Ö l s . Switchmg occurs at random between
two different conductance valucs The switchmg frequency
mcreases with mcreasmg bias voltage, äs shown in the
previous figure

related to the switching of a defect between two positions in the contact. The time τ, spend in a

Position* i (i =* l, 2) was successfully described by
the expression:

(1)

with* τ0ι* the attempt time of state* ι,* ε0ι the energy
barrier between the two metastable positions and

*ζ,* a parameter describing current induced
migra-tion of the defect [9]. Here* Td,* the defect

temperature, is expected to be larger than the environment temperature due to excitation by the current. Holweg et al. derived the expression

*Td = 5e\V\/I6kB* for the defect temperature in

the low temperature limit, which implies that the switching frequency increases with voltage.

In our contacts we interpret the Steps in the conductance äs being due to the displacement of an atom between two energetically equal posi-tions in the constriction region. The predicted increase of switching frequency for increasing bias, eq. (1), is also observed in our contacts, äs can be seen in fig. 6. The switching times of this TLF are shown äs a function of the inverse voltage in fig. 8. From this figure it appears that the attempt times TO( are äs high-äs 10~7s and

*that the barrier energies s0l/kB* are of the order

of 103 K. The energy barrier is comparable, but

the prefactors TO, are large compared to values

obtained in refs. [9,10].

An appropriate starting point for the

descrip-10° r

**T ( S )**

ΙΟ'2 μ

10"

10"

4.1 kO state

20 40 , . 6 0

Voltage '(V )

Fig 8 The average switchmg timcs äs a function of mverse voltage, äs obtamed at different bias currents for the two level fluctuations m fig 6 The straight lines are a fit to the data From the mtersection it appears that the attempt times T„, are äs high äs 10 7 s and from the slopes it follows that the

barner energies £„,/&„ are of the Order of 101 K.

tion of these contacts is the Landauer formula
*for the conductance G,*

2fl

*h* **H = l**

### Σ

* τ*

*η*

*,*

(2)
where* T„* is the transmission probability of
subband* n* and* Ν~^5/4π* is the total number
of occupied subbands. We have* S* = j-rrd and
A:F —ττ/α so that* N—(dla)2 (d* and* a* are the

constriction diameter and interatomic distance
respectively). Since* G* is only a few times* 2e l h*

we conclude that our contacts are of atomic
dimensions. Conductance quantization is
ob-served when the transmission probability of the
subbands is either unity or zero. Backscattering
of a subband destroys the quantization. In our
point contacts backscattering is likely, either
because of a rapidly varying potential or due to
impurities in the point contact region. The
re-markable aspect of the experiment is that the
displacement of a single atom can have an effect
of the order of* 2e2Ih* on the conductance. Since

in a metallic point contact the number of sub-bands is of the same order äs the number of atoms making up the contact, this finding is consistent with the notion of a conductance of

C* J Muller et al l Conductance and \upetcwient discontinuities in atomic size point contacts* 231

though no conductance quantization could be observed.

**4. Point contacts of superconducting niobium**

Superconducting electrodes are interesting because apart from the resistance an additional parameter, being the critical currcnt, can be studied. The product of the critical current 7C, and the normal resistance, 7?N, of a point contact represents a characteristic voltage of the order of

*Δ/e.* For a short weak link (äs compared to the
coherence length) Kulik and Omelyanchuk
showed that, in the classical limit of constriction
width much greater than Fermi wave length, the

*ICRN product is constant, independent ot RN.*

They analyzed two possible limits, a dirty contact where the electron mean free path is short compared to the constriction diameter [11] (KO-1) and a clean, ballistic, contact where the electron mean free path is much larger than the constriction diameter [12] (KO-2). In the zero temperature limit the calculated 7C7?N value for a

clean contact is* ττΔ/ε.* In a recent paper [4] it was

shown that this relation survives under
condi-tions that* RN* is quantized. As a result, 7L was

predicted to increase stepwise, äs a function of the constriction diameter, with Steps equal to

*eAlh.*

*We have measured a large number of I-V*
curves at 4.2 K, where the resistance is varied
over more than three Orders of magnitude, see
flg. 9. The normal resistance is derived from a
linear fit to the part of the curve between ±5 and
*±10 mV. For every point contact the ILRN*

prod-uct is thus obtained. These data points, together with the data of another MCB sample measured at 1.2 K, are given in fig. 10 äs a function of the normal resistance. Also indicated in this figure are the zero temperature predictions of Kulik and Omelyanchuk, KO-1 and KO-2 [11,12].

The Interpretation of this diagram is not yet clear to us. In the low resistance part of the diagram, below 80 Ω, it is suspected that heating

effects [13] or non-equilibrium effects [14] have their influence on the value of the 7C7?N product. An interesting part of fig. 10 is the resistance

DECREASINO CONSTRICTION

RADIUS

Fig 9 /—Kchaiactenstics of a niobium sample at 4 2 K The normal resistance is mcreased by dimimshmg the constriction radius, resultmg in a resistance change from approximately l Ω to l kil

ränge exceeding 80 Ω. In this ränge a uniform
*logarithmic decrease of the ICRN* product is

observed for two different samples at two differ-ent temperatures. One might think that for large normal resistances the 7C/?N product should be

232 *C J Müller et al l Conduclance and supercurrent ditLontinuities m atomic \ize point (antuet·.*

(mV)

sample 1

KO-2(clean)

KO-l(dirty)

sample 2 T=4.2 K

10"

*Fig 10 The 1^RN products äs d tunction of RN* on a

loganthmic scdle for two sdmples dt two difterent temperd-tures The predictions for the short dirty, KO-1, dnd the short clean, KO-2, wedk link are indicated At the Iow impedance side there is a steep increase in /CRN for

*decreas-ing RN At RN* vdlues exccedmg 80 il d uniform decrease of

7C/?N* for mcreasmg RN* is ohserved

their high normal resistance they are in the
*underdamped regime, ßL* S> 1. When a fluctuation

mechanism (thermal, electrical, quantum)
m-duces a System to switch to the voltage carrying
state before it has reached its maximum
theoreti-cal crititheoreti-cal current, the Iow dampmg will make it
easy for the System to remain there. Therefore, a
reduced damping together with a fluctuation
mechanism can explain the observed reduction
of 7C/?N* for increasing RN. However, that this*

decrease of the /C/?N* product at RN* values largcr

than 80 il has a logarithmic dependence remains to be explained.

*We now discuss the measurement of RN* and 7C

of atomic size niobium point contacts äs a function of continuously varying piezo voltage. The critical current is measured at a setpoint voltage near V = 0 , such that the critical current and the setpoint current coincide within 0.1%. The current biasing the sample is ramped until the setpoint voltage is reached. Then the set-point current value is held at an Output terminal while the current bias switches back to zero. This procedure is repeated periodically, which en-ables us to measure the critical current value while the constriction diameter is varied. For two periods of the piezo voltage such a measurement

1000 2000 3000 time(s)

Fig 11 A cnticdl cuircnt medsurement of d niobium Sdmple
over two periods of the tridngular piezo voltdge For an
mcreasmg constriction diameter (decreasing piezo voltagc)
Steps in critical current of the order of ε/1/7ι=04μΑ. are
observed The ditfercnce in the curvcs ror mcreasing and
decreasing* V* may rcflcct a dilference in strcss m the point
contact region

is presented in fig. 11. Clear critical current Steps
occur when the constriction diameter changes.
The step size is of the ordcr of* eA/ti* =0.4 μΑ,
consistent with the theoretical prediction of a
critical current* eAlh* per subband in a
supercon-ducting quantum point contact [4]. The slopes
for decreasing Vp are diflerent from those for
increasing Vp, which may be due to a different
stress in the point contact region when the
electrodes are moved apart compared to the
Situation where the electrodes are pressed into
each other. Although the rough shape of the two
slopes for increasing and decreasing Vp are
simi-lar, the detailed structure does not reproduce.
As in the case of the platinum contact wc expect
that in the used Vp amplitude of 80 V some
plastic deformation in the point contact region
occurs, so that the corresponding slopes do not
reproduce in detail.

In fig. 12 we show an analogous measurement

*äs in fig. 11 over three periods of Vp* with a

C* J Muller et al l Conductance and supercunent discontinuities in atomic size point contacts* 233

35 Ι.(μΑ)

3 2 5

700 600 500 (mV) l 75

165 60 Vp(V)

**50**

40

0 500 1000 , . 1500 time(s)

panels that this measurement reproduces
perfect-ly, even the fine structure of the* ICRN* product

reproduces with the period in Vp. This figure
shows that it is possible to move one or a few
atoms in a reproducible way in and out of a
constriction. The discontinuities in 7C line up
perfectly with the discontinuities in* RN* and* ICRN,*

äs can also be seen from fig. 13, which shows the

3 5

Α)

3

2 5

700

600

500

1.7

1.65 1000

time(s) 1500

Fig 12 Cntical current and normal resistance measurement
on a smaller piezo voltage ränge äs compared to fig 11 The
fine structure in 7C* lines up with that in RN and ICRN* The
*relatively large changes m Ii* and ΛΝ at the Steps almost

compensate each other m the product* ICRN*

resistance measurement is included, measured by
a lock-in amplifier at voltages larger than* 2Ale.*

This measurement is performed after the* Ic*

measurement with the same Vp scan, where the
minimum in* V* served äs a zero time reference.

The third panel shows the product of the 7C** and 5. Conclusions**

*the RN* values. It is clear from the top three

Fig 13 One period of fig 12 on an expanded scale

last period of fig. 12 on an expanded scale. The
variations of approximately 50% in 7C* and RN*

separately almost compensate and are reduced to about 7% variations in the product. The values of the 7C7?N product for the 7?N values considered

(500-750 Ω) with an average of 1.7 mV, are in

agreement with the values presented for two different samples in fig. 10.

234 *C ] Muller et al l Conductance and supercurrent discontinuüies in atomic size poml contacts*
well resolved Steps m the conductance

Applica-tion of the measurement technique to metals
with a large Fermi wave length compared to the
atomic dimensions (semimetals) may allow the
observation of conductance quantization We
have presented measurements on adjustable
point contacts of normal and superconducting
metals With the present technique it is possible
*to measure junction charactenstics, such äs IL*

and /C^N with the junction resistance äs a
param-eter When the constnction diamparam-eter is changed
a stepwise Variation m the cntical current is
observed, comcidmg with Steps m the
conduct-ance The steps m G and 7C are of the order of
*2e l h and εΔ/fi,* respectively

**Acknowledgement**

We wish to thank prof L J de Jongh for his interest and for stimulating discussions

**References**

[1] B J vanWees, H van Houten, C W J Beenakker, J G Williamson, L P Kouwenhoven, D van der Marel and C T Foxon Phys Rev Lett 60 (1988) 848,

D A Wharam T J Thornton R Newbury, M Pepper, H Ahmed, J E F Frost, D G Hasko, D C Peacock, D A Ritchie and G A C Jones, J Phys C 21 (1988) L209

[2] E A Montie E C Cosman, G W t Hooft, M B van der Mark and CWJ Beenakker, Nature 350 (1991) 594

[3] CWJ Beenakker and H van Houten, Solid State Phys 44 (1991) l

[4] CWJ Beenakker and H van Houten Phys Rev Lett 66 (1991) 3056,

CWJ Beenakker Phys Rev Lett 67(1991)3836 [5] C J Muller, J M van Ruitenbcek and L J de Jongh,

Physica C 191 (1992) 485

[6] C J Muller, J M van Ruitenbeek and L J de Jongh, Phys Rev Lett 69 (1992) 140

[7] J Moreland and J W Ekm, J Appl Phys 58 (1985) 3888

[8] Note that the atomic zero pomt Vibration amphtudes are much larger than the stabihty quoted here The atomic Vibration frequencies are of the Order of phonon fre quencies =10n Hz and the amphtudes are estimated to

be several picometers The expenmental frequency wmdow however, has its upper hmit at about 104 Hz,

implymg that in our expenmcnt the atomic positions are averaged over the Vibration amphtudes, which is only = 1% of the atomic size The referred stabihty is determmed by the observed random vanations of the resistance, i e electrode spacing, and therefore only sensitive to frequencies withm the expenmental wmdow [9] K S Ralls, D C Ralph and R A Buhrman, Phys Rev

B 40 (1989) 11561

[10] P A M Holweg, J Caro, A H Verbruggen and S Radelaar, Phys Rev B to be pubhshed

[11] I O Kuhk and A N Omelyanchuk, Pis'ma Zh Eksp Teor Fiz 21 (1975) 216 [JETP Lett 21 (1975) 96] [12] I O Kuhk and A N Omelyanchuk, Fiz Nizk Temp 3

(1977) 945 [Sov J Low Temp Phys 3 (1977) 459] [13] VN Gubankov, K K Likharev and N M Margolm,

Fiz Tverd Tela 14 (1972) 953 [Sov Phys-Solid State 14 (1972) 819],

T A Fulton and L N Dunklebcrgcr, J Appl Phys 45 (1974) 2283

[14] I K Yanson, personal communication

[15] V Ambegaokar and A Baratoff, Phys Rev Lett 10 (1963) 486, Phys Rev Lett 11 (1963) 104